#------------------------------------------------------------------------------
#$Date: 2025-07-01 13:44:59 +0300 (Tue, 01 Jul 2025) $
#$Revision: 1120 $
#$URL: svn://crystallography.net/testcod/cif/2/00/00/2000019.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2000019
loop_
_publ_author_name
'Strange, Nicholas A.'
'Bell, Robert T.'
'Park, James Eujin'
'Stone, Kevin H.'
'Coker, Eric N.'
'Ginley, David S.'
_publ_section_title
;
 Formation of Ba3Nb0.75Mn2.25O9-6H during thermochemical reduction of
 Ba4NbMn3O12-12R
;
_journal_issue                   5
_journal_name_full
'Acta Crystallographica Section E Crystallographic Communications'
_journal_page_first              469
_journal_page_last               473
_journal_paper_doi               10.1107/S2056989023003213
_journal_volume                  79
_journal_year                    2023
_chemical_formula_sum            'Ba4 Mn3 Nb O12'
_chemical_formula_weight         999.0213
_space_group_crystal_system      hexagonal
_space_group_IT_number           166
_space_group_name_Hall           '-R 3 2"'
_space_group_name_H-M_alt        'R -3 m :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   5.73256(3)
_cell_length_b                   5.73256(3)
_cell_length_c                   28.16620(19)
_cell_measurement_reflns_used    1248
_cell_measurement_temperature    300
_cell_measurement_theta_max      42
_cell_measurement_theta_min      4.25
_cell_volume                     801.597(8)
_diffrn_ambient_temperature      300
_diffrn_measured_fraction_theta_full 271
_diffrn_measurement_device_type  'SSRL beam line 2-1'
_diffrn_radiation_wavelength     0.729276500
_exptl_absorpt_coefficient_mu    20.215
_exptl_crystal_density_diffrn    6.20853(8)
_pd_block_diffractogram_id       Bell_BNM_scan1
_pd_block_id                     12R-barium_niobium_manganese_oxide
_pd_phase_name                   12R-Ba4NbMn3O12
_cod_data_source_file            wm5677sup3.txt
_cod_data_source_block           12R-barium_niobium_manganese_oxide
_cod_original_cell_volume        801.598(10)
_cod_original_sg_symbol_H-M      R-3m
_cod_original_formula_sum        Ba4NbMn3O12
_cod_database_code               2000019
loop_
_space_group_symop_id
_space_group_symop_operation_xyz
1 'x, y, z '
2 '-x, -y, -z '
3 '-x+y, -x, z '
4 '-x+y, y, z '
5 '-y, -x, z '
6 '-y, x-y, z '
7 'y, -x+y, -z '
8 'y, x, -z '
9 'x-y, -y, -z '
10 'x-y, x, -z '
11 '-x, -x+y, -z '
12 'x, x-y, z '
13 'x-1/3, y+1/3, z+1/3 '
14 '-x-1/3, -y+1/3, -z+1/3 '
15 '-x+y-1/3, -x+1/3, z+1/3 '
16 '-x+y-1/3, y+1/3, z+1/3 '
17 '-y-1/3, -x+1/3, z+1/3 '
18 '-y-1/3, x-y+1/3, z+1/3 '
19 'y-1/3, -x+y+1/3, -z+1/3 '
20 'y-1/3, x+1/3, -z+1/3 '
21 'x-y-1/3, -y+1/3, -z+1/3 '
22 'x-y-1/3, x+1/3, -z+1/3 '
23 '-x-1/3, -x+y+1/3, -z+1/3 '
24 'x-1/3, x-y+1/3, z+1/3 '
25 'x+1/3, y-1/3, z-1/3 '
26 '-x+1/3, -y-1/3, -z-1/3 '
27 '-x+y+1/3, -x-1/3, z-1/3 '
28 '-x+y+1/3, y-1/3, z-1/3 '
29 '-y+1/3, -x-1/3, z-1/3 '
30 '-y+1/3, x-y-1/3, z-1/3 '
31 'y+1/3, -x+y-1/3, -z-1/3 '
32 'y+1/3, x-1/3, -z-1/3 '
33 'x-y+1/3, -y-1/3, -z-1/3 '
34 'x-y+1/3, x-1/3, -z-1/3 '
35 '-x+1/3, -x+y-1/3, -z-1/3 '
36 'x+1/3, x-y-1/3, z-1/3 '
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_site_symmetry_multiplicity
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_B_iso_or_equiv
Ba1 Ba+2 6 0 0 0.12960(3) 1 0.61(9)
Ba2 Ba+2 6 0 0 0.28541(3) 1 0.61(9)
Nb3 Nb+5 3 0 0 0 1 0.43(8)
Mn1 Mn+4 3 0 0 0.5 1 0.43(8)
Mn5 Mn+3 6 0 0 0.41098(7) 1 0.43(8)
O1 O-2 18 0.47778 0.52222 0.12374(16) 1 0.65(10)
O2 O-2 18 0.50188 0.49812 0.29246(19) 1 0.65(10)
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
O1 Ba1 O1 51.107(4) 6_655 1_555 3_555
O1 Ba1 O1 119.674(13) 3_565 1_555 6_655
O1 Ba1 O1 169.02(8) 3_565 1_555 3_555
O1 Ba1 O1 68.674(5) 6_555 1_555 3_565
O1 Ba1 O1 169.02(8) 6_555 1_555 6_655
O1 Ba1 O1 119.674(13) 6_555 1_555 3_555
O1 Ba1 O1 119.674(13) 1_555 1_555 6_555
O1 Ba1 O1 51.107(4) 1_555 1_555 3_565
O1 Ba1 O1 68.674(5) 1_555 1_555 6_655
O1 Ba1 O1 119.674(13) 1_555 1_555 3_555
O1 Ba1 O1 169.02(8) 1_445 1_555 1_555
O1 Ba1 O1 51.107(4) 1_445 1_555 6_555
O1 Ba1 O1 119.674(13) 1_445 1_555 3_565
O1 Ba1 O1 119.674(13) 1_445 1_555 6_655
O1 Ba1 O1 68.674(5) 1_445 1_555 3_555
O1 Ba1 O1 57.86(14) 21_555 1_555 1_445
O1 Ba1 O1 124.82(4) 21_555 1_555 1_555
O1 Ba1 O1 57.86(14) 21_555 1_555 6_555
O1 Ba1 O1 95.34(7) 21_555 1_555 3_565
O1 Ba1 O1 124.82(4) 21_555 1_555 6_655
O1 Ba1 O1 95.34(7) 21_555 1_555 3_555
O1 Ba1 O1 67.29(9) 14_655 1_555 21_555
O1 Ba1 O1 95.34(7) 14_655 1_555 1_445
O1 Ba1 O1 95.34(7) 14_655 1_555 1_555
O1 Ba1 O1 124.82(4) 14_655 1_555 6_555
O1 Ba1 O1 124.82(4) 14_655 1_555 3_565
O1 Ba1 O1 57.86(14) 14_655 1_555 6_655
O1 Ba1 O1 57.86(14) 14_655 1_555 3_555
O1 Ba1 O1 67.29(9) 19_555 1_555 14_655
O1 Ba1 O1 67.29(9) 19_555 1_555 21_555
O1 Ba1 O1 124.82(4) 19_555 1_555 1_445
O1 Ba1 O1 57.86(14) 19_555 1_555 1_555
O1 Ba1 O1 95.34(7) 19_555 1_555 6_555
O1 Ba1 O1 57.86(14) 19_555 1_555 3_565
O1 Ba1 O1 95.34(7) 19_555 1_555 6_655
O1 Ba1 O1 124.82(4) 19_555 1_555 3_555
O2 Ba1 O1 107.01(8) 19_555 1_555 19_555
O2 Ba1 O1 144.91(4) 19_555 1_555 14_655
O2 Ba1 O1 144.91(4) 19_555 1_555 21_555
O2 Ba1 O1 113.78(10) 19_555 1_555 1_445
O2 Ba1 O1 57.24(10) 19_555 1_555 1_555
O2 Ba1 O1 89.66(8) 19_555 1_555 6_555
O2 Ba1 O1 57.24(10) 19_555 1_555 3_565
O2 Ba1 O1 89.66(8) 19_555 1_555 6_655
O2 Ba1 O1 113.78(10) 19_555 1_555 3_555
O2 Ba1 O2 56.64(9) 14_655 1_555 19_555
O2 Ba1 O1 144.91(4) 14_655 1_555 19_555
O2 Ba1 O1 107.01(8) 14_655 1_555 14_655
O2 Ba1 O1 144.91(4) 14_655 1_555 21_555
O2 Ba1 O1 89.66(8) 14_655 1_555 1_445
O2 Ba1 O1 89.66(8) 14_655 1_555 1_555
O2 Ba1 O1 113.78(10) 14_655 1_555 6_555
O2 Ba1 O1 113.78(10) 14_655 1_555 3_565
O2 Ba1 O1 57.24(10) 14_655 1_555 6_655
O2 Ba1 O1 57.24(10) 14_655 1_555 3_555
O2 Ba1 O2 56.64(9) 21_555 1_555 14_655
O2 Ba1 O2 56.64(9) 21_555 1_555 19_555
O2 Ba1 O1 144.91(4) 21_555 1_555 19_555
O2 Ba1 O1 144.91(4) 21_555 1_555 14_655
O2 Ba1 O1 107.01(8) 21_555 1_555 21_555
O2 Ba1 O1 57.24(10) 21_555 1_555 1_445
O2 Ba1 O1 113.78(10) 21_555 1_555 1_555
O2 Ba1 O1 57.24(10) 21_555 1_555 6_555
O2 Ba1 O1 89.66(8) 21_555 1_555 3_565
O2 Ba1 O1 113.78(10) 21_555 1_555 6_655
O2 Ba1 O1 89.66(8) 21_555 1_555 3_555
O1 Ba2 O1 69.71(10) 14_655 1_555 19_555
O1 Ba2 O1 69.71(10) 21_555 1_555 14_655
O1 Ba2 O1 69.71(10) 21_555 1_555 19_555
O2 Ba2 O1 92.73(8) 3_555 1_555 21_555
O2 Ba2 O1 58.93(11) 3_555 1_555 14_655
O2 Ba2 O1 128.62(11) 3_555 1_555 19_555
O2 Ba2 O2 172.0(2) 3_565 1_555 3_555
O2 Ba2 O1 92.73(8) 3_565 1_555 21_555
O2 Ba2 O1 128.62(11) 3_565 1_555 14_655
O2 Ba2 O1 58.93(11) 3_565 1_555 19_555
O2 Ba2 O2 59.098(11) 6_555 1_555 3_565
O2 Ba2 O2 119.53(3) 6_555 1_555 3_555
O2 Ba2 O1 58.93(11) 6_555 1_555 21_555
O2 Ba2 O1 128.62(11) 6_555 1_555 14_655
O2 Ba2 O1 92.73(8) 6_555 1_555 19_555
O2 Ba2 O2 172.0(2) 6_655 1_555 6_555
O2 Ba2 O2 119.53(3) 6_655 1_555 3_565
O2 Ba2 O2 60.586(11) 6_655 1_555 3_555
O2 Ba2 O1 128.62(11) 6_655 1_555 21_555
O2 Ba2 O1 58.93(11) 6_655 1_555 14_655
O2 Ba2 O1 92.73(8) 6_655 1_555 19_555
O2 Ba2 O2 119.53(3) 1_445 1_555 6_655
O2 Ba2 O2 60.586(11) 1_445 1_555 6_555
O2 Ba2 O2 119.53(3) 1_445 1_555 3_565
O2 Ba2 O2 59.098(11) 1_445 1_555 3_555
O2 Ba2 O1 58.93(11) 1_445 1_555 21_555
O2 Ba2 O1 92.73(8) 1_445 1_555 14_655
O2 Ba2 O1 128.62(11) 1_445 1_555 19_555
O2 Ba2 O2 172.0(2) 1_555 1_555 1_445
O2 Ba2 O2 59.098(11) 1_555 1_555 6_655
O2 Ba2 O2 119.53(3) 1_555 1_555 6_555
O2 Ba2 O2 60.586(11) 1_555 1_555 3_565
O2 Ba2 O2 119.53(3) 1_555 1_555 3_555
O2 Ba2 O1 128.62(11) 1_555 1_555 21_555
O2 Ba2 O1 92.73(8) 1_555 1_555 14_655
O2 Ba2 O1 58.93(11) 1_555 1_555 19_555
O2 Ba2 O2 114.91(6) 31_456 1_555 1_555
O2 Ba2 O2 57.34(15) 31_456 1_555 1_445
O2 Ba2 O2 86.91(9) 31_456 1_555 6_655
O2 Ba2 O2 86.91(9) 31_456 1_555 6_555
O2 Ba2 O2 114.91(6) 31_456 1_555 3_565
O2 Ba2 O2 57.34(15) 31_456 1_555 3_555
O2 Ba2 O1 116.17(7) 31_456 1_555 21_555
O2 Ba2 O1 116.17(7) 31_456 1_555 14_655
O2 Ba2 O1 172.49(9) 31_456 1_555 19_555
O2 Ba2 O2 57.58(10) 26_566 1_555 31_456
O2 Ba2 O2 86.91(9) 26_566 1_555 1_555
O2 Ba2 O2 86.91(9) 26_566 1_555 1_445
O2 Ba2 O2 114.91(6) 26_566 1_555 6_655
O2 Ba2 O2 57.34(15) 26_566 1_555 6_555
O2 Ba2 O2 57.34(15) 26_566 1_555 3_565
O2 Ba2 O2 114.91(6) 26_566 1_555 3_555
O2 Ba2 O1 116.17(7) 26_566 1_555 21_555
O2 Ba2 O1 172.49(9) 26_566 1_555 14_655
O2 Ba2 O1 116.17(7) 26_566 1_555 19_555
O2 Ba2 O2 57.58(10) 33_566 1_555 26_566
O2 Ba2 O2 57.58(10) 33_566 1_555 31_456
O2 Ba2 O2 57.34(15) 33_566 1_555 1_555
O2 Ba2 O2 114.91(6) 33_566 1_555 1_445
O2 Ba2 O2 57.34(15) 33_566 1_555 6_655
O2 Ba2 O2 114.91(6) 33_566 1_555 6_555
O2 Ba2 O2 86.91(9) 33_566 1_555 3_565
O2 Ba2 O2 86.91(9) 33_566 1_555 3_555
O2 Ba2 O1 172.49(9) 33_566 1_555 21_555
O2 Ba2 O1 116.17(7) 33_566 1_555 14_655
O2 Ba2 O1 116.17(7) 33_566 1_555 19_555
O2 Nb3 O2 90.19(18) 21_555 1_555 14_655
O2 Nb3 O2 89.81(18) 25_455 1_555 21_555
O2 Nb3 O2 180.000 25_455 1_555 14_655
O2 Nb3 O2 90.19(18) 27_565 1_555 25_455
O2 Nb3 O2 180.000 27_565 1_555 21_555
O2 Nb3 O2 89.81(18) 27_565 1_555 14_655
O2 Nb3 O2 89.81(18) 19_555 1_555 27_565
O2 Nb3 O2 89.81(18) 19_555 1_555 25_455
O2 Nb3 O2 90.19(18) 19_555 1_555 21_555
O2 Nb3 O2 90.19(18) 19_555 1_555 14_655
O2 Nb3 O2 180.00000000(8) 30_555 1_555 19_555
O2 Nb3 O2 90.19(18) 30_555 1_555 27_565
O2 Nb3 O2 90.19(18) 30_555 1_555 25_455
O2 Nb3 O2 89.81(18) 30_555 1_555 21_555
O2 Nb3 O2 89.81(18) 30_555 1_555 14_655
O1 Mn1 O1 97.07(16) 13_545 1_555 31_456
O1 Mn1 O1 180.00000000(4) 26_566 1_555 13_545
O1 Mn1 O1 82.93(16) 26_566 1_555 31_456
O1 Mn1 O1 97.07(16) 18_655 1_555 26_566
O1 Mn1 O1 82.93(16) 18_655 1_555 13_545
O1 Mn1 O1 180.000 18_655 1_555 31_456
O1 Mn1 O1 82.93(16) 15_555 1_555 18_655
O1 Mn1 O1 97.07(16) 15_555 1_555 26_566
O1 Mn1 O1 82.93(16) 15_555 1_555 13_545
O1 Mn1 O1 97.07(16) 15_555 1_555 31_456
O1 Mn1 O1 180.00000000(4) 33_566 1_555 15_555
O1 Mn1 O1 97.07(16) 33_566 1_555 18_655
O1 Mn1 O1 82.93(16) 33_566 1_555 26_566
O1 Mn1 O1 97.07(16) 33_566 1_555 13_545
O1 Mn1 O1 82.93(16) 33_566 1_555 31_456
Mn5 Mn1 O1 49.87(11) 2_556 1_555 33_566
Mn5 Mn1 O1 130.13(11) 2_556 1_555 15_555
Mn5 Mn1 O1 130.13(11) 2_556 1_555 18_655
Mn5 Mn1 O1 49.87(11) 2_556 1_555 26_566
Mn5 Mn1 O1 130.13(11) 2_556 1_555 13_545
Mn5 Mn1 O1 49.87(11) 2_556 1_555 31_456
Mn5 Mn1 Mn5 180.000 1_555 1_555 2_556
Mn5 Mn1 O1 130.13(11) 1_555 1_555 33_566
Mn5 Mn1 O1 49.87(11) 1_555 1_555 15_555
Mn5 Mn1 O1 49.87(11) 1_555 1_555 18_655
Mn5 Mn1 O1 130.13(11) 1_555 1_555 26_566
Mn5 Mn1 O1 49.87(11) 1_555 1_555 13_545
Mn5 Mn1 O1 130.13(11) 1_555 1_555 31_456
O1 Mn5 O1 79.89(16) 13_545 1_555 15_555
O1 Mn5 O1 79.89(16) 18_655 1_555 13_545
O1 Mn5 O1 79.89(16) 18_655 1_555 15_555
O2 Mn5 O1 92.18(12) 26_566 1_555 18_655
O2 Mn5 O1 169.60(18) 26_566 1_555 13_545
O2 Mn5 O1 92.18(12) 26_566 1_555 15_555
O2 Mn5 O2 94.85(19) 33_566 1_555 26_566
O2 Mn5 O1 92.18(12) 33_566 1_555 18_655
O2 Mn5 O1 92.18(12) 33_566 1_555 13_545
O2 Mn5 O1 169.60(18) 33_566 1_555 15_555
O2 Mn5 O2 94.85(19) 31_456 1_555 33_566
O2 Mn5 O2 94.85(19) 31_456 1_555 26_566
O2 Mn5 O1 169.60(18) 31_456 1_555 18_655
O2 Mn5 O1 92.18(12) 31_456 1_555 13_545
O2 Mn5 O1 92.18(12) 31_456 1_555 15_555
Mn1 Mn5 O2 121.75(14) 1_555 1_555 31_456
Mn1 Mn5 O2 121.75(14) 1_555 1_555 33_566
Mn1 Mn5 O2 121.75(14) 1_555 1_555 26_566
Mn1 Mn5 O1 47.85(11) 1_555 1_555 18_655
Mn1 Mn5 O1 47.85(11) 1_555 1_555 13_545
Mn1 Mn5 O1 47.85(11) 1_555 1_555 15_555
Mn5 O1 Mn1 82.28(4) 25_565 1_555 25_565
O1 O1 Mn5 50.06(8) 6_665 1_555 25_565
O1 O1 Mn1 48.54(8) 6_665 1_555 25_565
O1 O1 O1 60.000 3_565 1_555 6_665
O1 O1 Mn5 50.06(8) 3_565 1_555 25_565
O1 O1 Mn1 48.54(8) 3_565 1_555 25_565
O1 O1 O1 63.78(8) 19_555 1_555 3_565
O1 O1 O1 90.000 19_555 1_555 6_665
O1 O1 Mn5 112.84(4) 19_555 1_555 25_565
O1 O1 Mn1 41.46(8) 19_555 1_555 25_565
O1 O1 O1 52.44(17) 21_665 1_555 19_555
O1 O1 O1 90.000 21_665 1_555 3_565
O1 O1 O1 63.78(8) 21_665 1_555 6_665
O1 O1 Mn5 112.84(4) 21_665 1_555 25_565
O1 O1 Mn1 41.46(8) 21_665 1_555 25_565
O2 O1 O1 115.60(8) 21_665 1_555 21_665
O2 O1 O1 152.56(3) 21_665 1_555 19_555
O2 O1 O1 94.227(9) 21_665 1_555 3_565
O2 O1 O1 63.78(6) 21_665 1_555 6_665
O2 O1 Mn5 44.39(8) 21_665 1_555 25_565
O2 O1 Mn1 111.88(7) 21_665 1_555 25_565
O2 O1 O2 62.06(14) 19_555 1_555 21_665
O2 O1 O1 152.56(3) 19_555 1_555 21_665
O2 O1 O1 115.60(8) 19_555 1_555 19_555
O2 O1 O1 63.78(6) 19_555 1_555 3_565
O2 O1 O1 94.227(9) 19_555 1_555 6_665
O2 O1 Mn5 44.39(8) 19_555 1_555 25_565
O2 O1 Mn1 111.88(7) 19_555 1_555 25_565
Ba2 O1 O2 61.09(10) 14_655 1_555 19_555
Ba2 O1 O2 61.09(10) 14_655 1_555 21_665
Ba2 O1 O1 144.544(16) 14_655 1_555 21_665
Ba2 O1 O1 144.544(16) 14_655 1_555 19_555
Ba2 O1 O1 124.85(5) 14_655 1_555 3_565
Ba2 O1 O1 124.85(5) 14_655 1_555 6_665
Ba2 O1 Mn5 89.14(16) 14_655 1_555 25_565
Ba2 O1 Mn1 171.42(17) 14_655 1_555 25_565
Ba1 O1 Ba2 89.57(6) 1_555 1_555 14_655
Ba1 O1 O2 63.30(7) 1_555 1_555 19_555
Ba1 O1 O2 125.24(15) 1_555 1_555 21_665
Ba1 O1 O1 114.20(18) 1_555 1_555 21_665
Ba1 O1 O1 61.997(16) 1_555 1_555 19_555
Ba1 O1 O1 64.4466(18) 1_555 1_555 3_565
Ba1 O1 O1 124.337(3) 1_555 1_555 6_665
Ba1 O1 Mn5 95.47(6) 1_555 1_555 25_565
Ba1 O1 Mn1 91.24(7) 1_555 1_555 25_565
Ba1 O1 Ba1 169.02(8) 1_665 1_555 1_555
Ba1 O1 Ba2 89.57(6) 1_665 1_555 14_655
Ba1 O1 O2 125.24(15) 1_665 1_555 19_555
Ba1 O1 O2 63.30(7) 1_665 1_555 21_665
Ba1 O1 O1 61.997(16) 1_665 1_555 21_665
Ba1 O1 O1 114.20(18) 1_665 1_555 19_555
Ba1 O1 O1 124.337(3) 1_665 1_555 3_565
Ba1 O1 O1 64.4466(18) 1_665 1_555 6_665
Ba1 O1 Mn5 95.47(6) 1_665 1_555 25_565
Ba1 O1 Mn1 91.24(7) 1_665 1_555 25_565
Ba1 O1 Ba1 84.66(7) 14_655 1_555 1_665
Ba1 O1 Ba1 84.66(7) 14_655 1_555 1_555
Ba1 O1 Ba2 98.934(14) 14_655 1_555 14_655
Ba1 O1 O2 140.71(3) 14_655 1_555 19_555
Ba1 O1 O2 140.71(3) 14_655 1_555 21_665
Ba1 O1 O1 60.14(13) 14_655 1_555 21_665
Ba1 O1 O1 60.14(13) 14_655 1_555 19_555
Ba1 O1 O1 123.65(5) 14_655 1_555 3_565
Ba1 O1 O1 123.65(5) 14_655 1_555 6_665
Ba1 O1 Mn5 171.93(16) 14_655 1_555 25_565
Ba1 O1 Mn1 89.64(17) 14_655 1_555 25_565
Nb3 O2 Mn5 176.62(11) 13_655 1_555 26_566
O1 O2 Nb3 139.11(11) 21_665 1_555 13_655
O1 O2 Mn5 43.44(10) 21_665 1_555 26_566
O1 O2 O1 52.43(12) 19_555 1_555 21_665
O1 O2 Nb3 139.11(11) 19_555 1_555 13_655
O1 O2 Mn5 43.44(10) 19_555 1_555 26_566
O2 O2 O1 123.61(7) 33_566 1_555 19_555
O2 O2 O1 175.43(12) 33_566 1_555 21_665
O2 O2 Nb3 45.09(9) 33_566 1_555 13_655
O2 O2 Mn5 132.47(10) 33_566 1_555 26_566
O2 O2 O2 60.2(2) 31_566 1_555 33_566
O2 O2 O1 175.43(12) 31_566 1_555 19_555
O2 O2 O1 123.61(7) 31_566 1_555 21_665
O2 O2 Nb3 45.09(9) 31_566 1_555 13_655
O2 O2 Mn5 132.47(10) 31_566 1_555 26_566
O2 O2 O2 90.000 6_655 1_555 31_566
O2 O2 O2 59.89(11) 6_655 1_555 33_566
O2 O2 O1 94.227(9) 6_655 1_555 19_555
O2 O2 O1 121.03(7) 6_655 1_555 21_665
O2 O2 Nb3 44.91(9) 6_655 1_555 13_655
O2 O2 Mn5 137.43(10) 6_655 1_555 26_566
O2 O2 O2 60.000 3_665 1_555 6_655
O2 O2 O2 59.89(11) 3_665 1_555 31_566
O2 O2 O2 90.000 3_665 1_555 33_566
O2 O2 O1 121.03(7) 3_665 1_555 19_555
O2 O2 O1 94.227(9) 3_665 1_555 21_665
O2 O2 Nb3 44.91(9) 3_665 1_555 13_655
O2 O2 Mn5 137.43(10) 3_665 1_555 26_566
Ba2 O2 O2 60.451(5) 1_665 1_555 3_665
Ba2 O2 O2 120.293(5) 1_665 1_555 6_655
Ba2 O2 O2 63.755(18) 1_665 1_555 31_566
Ba2 O2 O2 124.0(2) 1_665 1_555 33_566
Ba2 O2 O1 112.40(15) 1_665 1_555 19_555
Ba2 O2 O1 59.98(7) 1_665 1_555 21_665
Ba2 O2 Nb3 92.58(5) 1_665 1_555 13_655
Ba2 O2 Mn5 87.60(7) 1_665 1_555 26_566
Ba2 O2 Ba2 172.0(2) 1_555 1_555 1_665
Ba2 O2 O2 120.293(5) 1_555 1_555 3_665
Ba2 O2 O2 60.451(5) 1_555 1_555 6_655
Ba2 O2 O2 124.0(2) 1_555 1_555 31_566
Ba2 O2 O2 63.755(18) 1_555 1_555 33_566
Ba2 O2 O1 59.98(7) 1_555 1_555 19_555
Ba2 O2 O1 112.40(15) 1_555 1_555 21_665
Ba2 O2 Nb3 92.58(5) 1_555 1_555 13_655
Ba2 O2 Mn5 87.60(7) 1_555 1_555 26_566
O2 O2 Ba2 59.707(5) 3_565 1_555 1_555
O2 O2 Ba2 119.549(5) 3_565 1_555 1_665
O2 O2 O2 180.000 3_565 1_555 3_665
O2 O2 O2 120.000 3_565 1_555 6_655
O2 O2 O2 120.11(11) 3_565 1_555 31_566
O2 O2 O2 90.000 3_565 1_555 33_566
O2 O2 O1 58.97(7) 3_565 1_555 19_555
O2 O2 O1 85.773(9) 3_565 1_555 21_665
O2 O2 Nb3 135.09(9) 3_565 1_555 13_655
O2 O2 Mn5 42.57(10) 3_565 1_555 26_566
O2 O2 O2 60.000 6_665 1_555 3_565
O2 O2 Ba2 119.549(5) 6_665 1_555 1_555
O2 O2 Ba2 59.707(5) 6_665 1_555 1_665
O2 O2 O2 120.000 6_665 1_555 3_665
O2 O2 O2 180.000 6_665 1_555 6_655
O2 O2 O2 90.000 6_665 1_555 31_566
O2 O2 O2 120.11(11) 6_665 1_555 33_566
O2 O2 O1 85.773(9) 6_665 1_555 19_555
O2 O2 O1 58.97(7) 6_665 1_555 21_665
O2 O2 Nb3 135.09(9) 6_665 1_555 13_655
O2 O2 Mn5 42.57(10) 6_665 1_555 26_566
Ba1 O2 O2 118.32(5) 14_655 1_555 6_665
Ba1 O2 O2 118.32(5) 14_655 1_555 3_565
Ba1 O2 Ba2 86.89(10) 14_655 1_555 1_555
Ba1 O2 Ba2 86.89(10) 14_655 1_555 1_665
Ba1 O2 O2 61.68(5) 14_655 1_555 3_665
Ba1 O2 O2 61.68(5) 14_655 1_555 6_655
Ba1 O2 O2 121.56(7) 14_655 1_555 31_566
Ba1 O2 O2 121.56(7) 14_655 1_555 33_566
Ba1 O2 O1 59.46(11) 14_655 1_555 19_555
Ba1 O2 O1 59.46(11) 14_655 1_555 21_665
Ba1 O2 Nb3 91.92(8) 14_655 1_555 13_655
Ba1 O2 Mn5 91.46(19) 14_655 1_555 26_566
Ba2 O2 Ba1 179.43(12) 26_566 1_555 14_655
Ba2 O2 O2 61.21(5) 26_566 1_555 6_665
Ba2 O2 O2 61.21(5) 26_566 1_555 3_565
Ba2 O2 Ba2 93.09(9) 26_566 1_555 1_555
Ba2 O2 Ba2 93.09(9) 26_566 1_555 1_665
Ba2 O2 O2 118.79(5) 26_566 1_555 3_665
Ba2 O2 O2 118.79(5) 26_566 1_555 6_655
Ba2 O2 O2 58.91(16) 26_566 1_555 31_566
Ba2 O2 O2 58.91(16) 26_566 1_555 33_566
Ba2 O2 O1 120.05(4) 26_566 1_555 19_555
Ba2 O2 O1 120.05(4) 26_566 1_555 21_665
Ba2 O2 Nb3 88.65(19) 26_566 1_555 13_655
Ba2 O2 Mn5 87.97(8) 26_566 1_555 26_566
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
Ba1 O1 2.87949(19) 1_555 3_555
Ba1 O1 2.87949(19) 1_555 6_655
Ba1 O1 2.87949(19) 1_555 3_565
Ba1 O1 2.87949(19) 1_555 6_555
Ba1 O1 2.87949(19) 1_555 1_555
Ba1 O1 2.87949(19) 1_555 1_445
Ba1 O1 2.932(4) 1_555 21_555
Ba1 O1 2.932(4) 1_555 14_655
Ba1 O1 2.932(4) 1_555 19_555
Ba1 O2 2.987(5) 1_555 19_555
Ba1 O2 2.987(5) 1_555 14_655
Ba1 O2 2.987(5) 1_555 21_555
Ba2 O1 2.842(4) 1_555 19_555
Ba2 O1 2.842(4) 1_555 14_655
Ba2 O1 2.842(4) 1_555 21_555
Ba2 O2 2.8732(5) 1_555 3_555
Ba2 O2 2.8732(5) 1_555 3_565
Ba2 O2 2.8732(5) 1_555 6_555
Ba2 O2 2.8732(5) 1_555 6_655
Ba2 O2 2.8732(5) 1_555 1_445
Ba2 O2 2.8732(5) 1_555 1_555
Ba2 O2 3.009(5) 1_555 31_456
Ba2 O2 3.009(5) 1_555 26_566
Ba2 O2 3.009(5) 1_555 33_566
Nb3 O2 2.001(3) 1_555 14_655
Nb3 O2 2.001(3) 1_555 21_555
Nb3 O2 2.001(3) 1_555 25_455
Nb3 O2 2.001(3) 1_555 27_565
Nb3 O2 2.001(3) 1_555 19_555
Nb3 O2 2.001(3) 1_555 30_555
Mn1 O1 1.876(3) 1_555 31_456
Mn1 O1 1.876(3) 1_555 13_545
Mn1 O1 1.876(3) 1_555 26_566
Mn1 O1 1.876(3) 1_555 18_655
Mn1 O1 1.876(3) 1_555 15_555
Mn1 O1 1.876(3) 1_555 33_566
Mn1 Mn5 2.5074(18) 1_555 2_556
Mn1 Mn5 2.5074(18) 1_555 1_555
Mn5 O1 1.935(3) 1_555 15_555
Mn5 O1 1.935(3) 1_555 13_545
Mn5 O1 1.935(3) 1_555 18_655
Mn5 O2 1.968(3) 1_555 26_566
Mn5 O2 1.968(3) 1_555 33_566
Mn5 O2 1.968(3) 1_555 31_456
Mn5 Mn1 2.5074(18) 1_555 1_555
O1 Mn1 1.876(3) 1_555 25_565
O1 Mn5 1.935(3) 1_555 25_565
O1 O1 2.484149(12) 1_555 6_665
O1 O1 2.484149(12) 1_555 3_565
O1 O1 2.811(8) 1_555 19_555
O1 O1 2.811(8) 1_555 21_665
O1 O2 2.812(6) 1_555 21_665
O1 O2 2.812(6) 1_555 19_555
O1 Ba2 2.842(4) 1_555 14_655
O1 Ba1 2.87949(19) 1_555 1_555
O1 Ba1 2.87949(19) 1_555 1_665
O1 Ba1 2.932(4) 1_555 14_655
O2 Mn5 1.968(3) 1_555 26_566
O2 Nb3 2.001(3) 1_555 13_655
O2 O1 2.812(6) 1_555 21_665
O2 O1 2.812(6) 1_555 19_555
O2 O2 2.825(9) 1_555 33_566
O2 O2 2.825(9) 1_555 31_566
O2 O2 2.833950(14) 1_555 6_655
O2 O2 2.833950(14) 1_555 3_665
O2 Ba2 2.8732(5) 1_555 1_665
O2 Ba2 2.8732(5) 1_555 1_555
O2 O2 2.898613(15) 1_555 3_565
O2 O2 2.898613(15) 1_555 6_665
O2 Ba1 2.987(5) 1_555 14_655
O2 Ba2 3.009(5) 1_555 26_566
